2Introduction Wood fibers swell under the influence of water. Thus, the dimensions and shape of paper or board change with change in moisture content.Poor dimensional stability causes many problems including misregister in multicolor printing, curl, cockling, wavy edges and asymmetric shrinkage in fusers of laser printers and copiers and during drying of ink on press.We consider the control of moisture content and relate moisture change to dimensional changes.
3Moisture in paperIn equilibrium, the moisture content of paper depends on temperature and partial vapor pressure of water (i.e. on relative humidity).The moisture content is highest in humid cold conditions.Pulp composition effects the moisture content of paper.The fiber wall structure changes when water is removed.Depending on pulp type, these changes may be partially irreversible.
4Relative humidityThe relative humidity of air is defined in terms of the vapor pressure of water.We denote the water vapor pressure as Pw and the saturation vapor pressure as Pws.At a given temperature below the critical temperature, Pws is the pressure at which water vapor is in equilibrium with liquid water.Pws must increase with temperature, since more hydrogen bonds break on heating.The relative humidity is defined asRH=Pw / Pws
5The relationship between temperature, relative humidity and water vapor pressure is given in Figure 1.Wood fibers are hygroscopic, i.e. they absorb water readily.The moisture content is absorbed mass of water/ mass of oven dry paper.The moisture content decreases with increasing temperature or with decreasing relative humidity.
6The effect of moisture content on temperature and relative humidity are shown in Figure 2. Mechanical pulps contain more moisture than chemical pulps (Figure 3).Fines are more important for moisture in mechanical pulps.Amorphous cellulose and hemicellulose are more important for chemical pulp moisture.
7Hysteresis and dynamic phenomena The effects of hysteresis on moisture content are that the moisture content of paper at a given relative humidity is different in absorption from dry conditions than in desorption from humid conditions.This is clearly evident in Figure 3.A pair of boundary curves is given in Figure 4.Depending upon the humidity history, the moisture content can be anywhere between the boundary curves.
8The difference in moisture content at fixed RH & T becomes large at high humidity or low temperature.Thermal energy, or heat of desorption, is necessary to remove water from fibers and the heat of adsorption releases when water adsorbs on fibers.Hysteresis is not a dynamic effect and the loop does not collapse even if moisture content changes very slowly.This is in part due to capillary condensation, whereby liquid water is trapped in pores.
9Another explanation is based on swelling stresses. Swelling stresses arise in the fiber wall because crystalline cellulose doesn't swell.At small amounts of water, the deformations are reversible and elastic.At larger amounts of water, the swelling stress may exceed a yield limit and cause plastic deformations.Weakly bonded micelles may free more OH groups to absorb water.
10Dynamic phenomenaThe diffusion time of moisture into paper is proportional to basis weight squared for relatively high basis weight paper.The diffusion time is proportional to basis weight for low basis weight paper.This is characteristic of boundary layer formation at the sheet surface.In the boundary layer, the local humidity and temperature differ from the ambient conditions.The heat of sorption governs the conditions in the boundary layer.
11With moisture adsorption, temperature increases and RH decreases in the boundary layer. This retards the diffusion process because the relative humidity seen by the sheet surface is lower than the ambient RH.The sorption rate increases if heat exchanges effectively between paper and its surroundings (air blows).Sometimes dimensional stability problems occur when opening a moisture sealed package where the vapor pressure differs from that of the surrounding air.
12Interaction of water with fibers The amount of absorbed water is a small fraction of the dry mass that the paper has when dried in an oven.On the other extreme, the water content of a wet pulp can be higher than the dry mass.Solids content, the ratio of dry mass to the total mass, gives the water content in cases such as a wet paper web.The water retention value (WRV) of a pulp is a common measure of total amount of water retained by a wet pulp.
13Fibers absorb water either as free water Inter-fiber free water in the pores, orIntra-fiber free water in the lumen of fibers,or as bound waterFreezing bound water in the pores of the fiber wall orNonfreezing bound water, chemically bonded to the hydroxylic and carboxylic acid groups in fibers.
14Figure 5 shows shows the proportions of water in the drying of TMP. Only water molecules bound to hydroxyl groups remain in fibers at moisture contents below 20%.The pores of a fiber wall are active when moisture content is 20-40% or RH > 90% at T=23°C.Free water is significant only at higher moisture content.
15Differential scanning calorimetry can resolve the fractions of free and bound water. The solute exclusion technique gives information about the distribution of water in the pores of the fiber wall.With this technique, pores are filled with macromolecules of different sizes.As the molecular size increases, the volume accessible to them decreases.Water fills the remaining pores and eventually reaches saturation.This is called the fiber saturation point.
16Fibers swell upon water absorption because water molecules penetrate between hydrogen bonded fibrils in the fiber wall as shown in Figure 6.The phenomenon, called Hornification refers to the irreversible loss of water absorption capacity in drying.On rewetting, the once dried pulp absorbs less water than before drying.
17Hornification only occurs in chemical pulps. It probably arises from the irreversible collapse of pores between fibrils indicated from D to B in Figure 6.Beating can partially reverse hornification.Cellulose and hemicellulose contain three OH groups per six carbon atoms.Lignin contains one or two OH per 10 carbon atoms.In amorphous hemicellulose, internal bond is weak, OH available for water.
18In crystalline cellulose, bonding is strong, OH are not available for hydrogen bonding with water. Figure 7 summarizes the removal of water from fibers during the different phases of papermaking, along with the changes in fiber cross section.The cross section is important because most shrinkage of paper comes from the transverse shrinkage of fibers.Paper starts to shrink at 50-60% solids.
19HygroexpansionWe will outline the hygroexpansion phenomena that are relevant for different papers.We will relate the hygroexpansivity of paper to the microscopic structure of the fiber network.We also consider the effects of hygroexpansivity on furnish composition and control variables in the papermaking process.
20General phenomenaThe hygroexpansive strain, eh, of paper is the incremental change in dimensions when the moisture content changes in the either the MD or CD.eh is a linear reversible function of the moisture content as seen in Figure 8.The hygroexpansivity is defined as=h/mcwhere b is the hygroexpansivity and Dmc is the change in moisture content.
21In the reversible region, b is independent of the actual moisture content change. When plotted against relative humidity, the hygroexpansive strains are generally nonlinear.Figure 9 shows the same data as Figure 8, except that RH is the x axis.Hysteresis results from the moisture content- relative humidity relationship.The strain values at given RH are different in adsorption and desorption.
22The slope, deh/dRH is different in the two directions. The internal stresses of paper release when moisture content increases sufficiently.As a result, paper shrinks irreversibly if it was initially dried under restraint as shown in Figure 8.Freely dried paper shows no irreversible shrinkage.In machine made papers, hygroexpansion is different in MD and CD.
23CD=0.1-0.15 is typically 3-5 times larger than in MD. z is one or two orders of magnitude larger than in MD and CD.The wet expansion of paper is important in offset printing, where approximately 1g/m2 is applied to the paper surface.Typical wet expansion of 1-2% is clearly larger than hygroexpansion.In printing, the time dependence of dimensional changes is often more important than the magnitude of the change.
24Hygroexpansion of the Fiber Network Over the 0-100% range of RH at room temperature, cellulosic fibrils expand approximately 1% in the longitudinal direction and approximately 20% in the transverse direction.The corresponding hygroexpansion coefficients of fibers are bLf=.03 and bTf=.6.Uesaka showed that the machine direction hygroexpansion coefficient is given bybMD=bLf+f21bTf
25The corresponding expression for the cross direction is bCD=bLf+f22bTfbLf and bTf are the longitudinal and transverse hygroexpansion coefficients of fiber,f2j describes the transfer of stress from direction j (j=1 for MD and 2 for CD) in the network to the transverse direction of a single fiber.The relative importance of the jf depends on the stress transfer parameters f2j, that are in turn determined by the inter-fiber bonds.
26Numerical calculations by Uesaka and Qi (our own Dewei Qi) suggested that in a lap joint bond, such as shown in Figure 10a, the transfer is very ineffective and f2j<<1.The “wrapped-around” in Figure 10b was shown to give a much larger transfer factor f2j.The MD hygroexpansivity of paper, bMD, is at most slightly larger than the average axial hygroexpansivity of fibers, bTf.The RBA has only a small effect.
27Figure 11 corroborates this, since the higher paper density has little effect on bMD. Wrapped-around bonds probably form primarily by fibers in the CD.In a MD fiber, wet strain and drying stress straighten undulations.Stress transfer is effective in compressed fiber segment and “wrapped-around” bonds.Figure 11 shows that higher fiber orientations increase hygroexpansion in CD, but not in CD.
28Drying stressesDrying shrinkage of paper presumably leads to the wrap-around geometry of Figure 10b.This bonding geometry explains why drying shrinkage has a strong effect on the hygroexpansion of paper.If the drying shrinkage of a pulp varies, the hygroexpansivity is approximately linear in the drying shrinkage as shown in Figure 12.
29Nonzero hygroexpansion occurs in fully restrained drying. The effect of wet straining depends on the solids content at which the strain is applied as shown in Figure 12.If paper is strained at a high solids content, hygroexpansion decreases linearly with increasing wet strain.The CD shrinkage is smallest at the center of the web.The CD hygroexpansivity is larger at the edges of the web as shown in Figure 13.